# Review from Mechanical Properties of Materials Concept of Stress and Strain

CIE 361 Fall 2004 Instructor: Christine Human

## Review from Mechanical Properties of Materials

### Concept of Stress and Strain

Figure 1 shows the behavior of a cylindrical body subjected to tension and compression. • • Tension specimen extends along its axis and contracts on the orthogonal (circumferential) axes Compression specimen compresses along its axis and expands on the orthogonal (circumferential) axes x y z

Figure 1:

Specimen under tension and compression (Callister(2000))

Axial stress

(units of psi or MPa) is the applied axial load

P

divided by the original cross sectional area,

A

0 : σ

x

=

P A

0 (1)

Axial strain

(dimensionless, in/in, m/m) relates the change in length of the specimen to the original length. It is calculated as follows: ε

x

= ∆

l

0

l

=

l

l

0

l

0 where ε

l

0

x

is the original length is the axial strain During a tension test the sample will elongate, therefore

l

positive. >

l

0 and the strain will be 9/24/2004 1

CIE 361 Fall 2004 Instructor: Christine Human

### Mechanical Properties of Material

Certain mechanical properties of the material can be determined from a plot of stress against strain.

Modulus of Elasticity

In the linear elastic range of response, the stress is proportional to the strain as shown in Figure 2 below. Unload Slope=E=modulus of elasticity Load Strain

Figure 2:

Initial portion of stress-strain curve The relationship is written as:

E

= σ ε Hooke’s Law where E is known as the

modulus of elasticity

or

Young’s modulus

. Typical values of

E

for steel, aluminum and titanium are given in Table 1.

Table 1:

Typical values of modulus of elasticity Modulus of elasticity,

E

Metal GPa ksi Steel 207 30000 Aluminum 69 10000 Titanium 115 16500 The largest value of the stress for which Hooke’s law can be used for a given material is known as the proportional limit, P L , of that material. It marks the change from linear elastic behavior to non-linear elastic behavior (see Figure 3). 9/24/2004 2

CIE 361 Fall 2004 Instructor: Christine Human

Yielding and yield strength

The yield point marks the transition from essentially elastic behavior (strain is recoverable upon unloading) to plastic behavior (some permanent deformation upon unloading). Some metals (including mild steel) exhibit the stress-strain relationship shown in Figure 3, part (a) where the yield point is clearly defined. In this figure, the yield point and the proportional limit coincide. The elastic to plastic transition is well defined by an

upper yield

point. However, for such materials the yield strength is taken as the average strength associated with the

lower yield

point. For metals exhibiting a stress-strain relationship similar to that shown in part (b), with no well defined yield point, the 0.2% offset strain is used to determine the yield strength. The yield strength is typically denoted as σ

y

. Upper yield point and P L σ Y P L σ Y Lower yield point strain strain 0.2% offset (a) (b)

Figure 3:

Yield Point

Plastic Behavior

As a metal deforms past its yield point, plastic deformations will result. Plastic deformation is associated with slip in crystalline materials such as metals (you will talk about this more in CIE 327). The process is not reversible.

Tensile strength

After yielding, the stress necessary to increase deformation increases to a maximum, shown as point

M

in Figure 4. Also shown in this figure are the states of deformation of a test specimen at various points along the stress-strain curve. The maximum stress is termed the tensile strength, typically denotes as σ

u

. 9/24/2004 3

CIE 361 Fall 2004 Instructor: Christine Human

Figure 4:

Stress-Strain curve to failure (Callister (2000)

)

Breaking Strength

Point F in Figure 4 corresponds to the breaking (or fracture) strength.

Ductility

Ductility is a measure of the plastic deformation capacity of a metal. Consider Figure 5 below:

Figure 5

: Brittle and ductile behavior (from Callister) A brittle (opposite of ductile) material is one with limited (or no) plastic deformation capacity. One metric for brittleness is a fracture strain of 5% or less. 9/24/2004 4

CIE 361 Fall 2004 Instructor: Christine Human A measure of ductility can be obtained by calculating either % elongation or % reduction in area. The percent elongation is the percentage of plastic strain at fracture and is given by %

EL

=

l f

l

0

l

0 100 (3) where

l f

is the fracture length. When reporting %

EL

, the original gage length (often 2 in or 50 mm) must also be reported. For commonly used steels, the specified minimum elongation is 21%. % reduction in area is calculated from the following equation: %

AR

=

A

0 −

A

0

A f

100 High values of %AR indicate necking of the specimen and ductile behavior. Typical values for structural steel are 60 to 70%. Table 2 below gives values of yield strength, tensile strength and ductility for mild steel, aluminum and titanium.

Table 2:

Typical values of yield strength, tensile strength and ductility Yield Tensile Metal MPa ksi MPA Ductility %

EL

Structural Steel Aluminum (6061) 248 36 400 58 21% 240 35 260 38 17% Titanium 830 120 900 130 10%

Strain Energy

The work done by the load P as it is slowly applied to the specimen results in an increase in stored energy associated with deformation of the rod. This energy is referred to as the strain energy of the rod. Strain Energy =

U

=

x

1 ∫ 0

Pdx

(4) which is equal to the area under the load deformation diagram between x=0 and x=x 1 as shown in Figure 6 9/24/2004 5

CIE 361 Fall 2004 P Instructor: Christine Human

## U=Area

P x x x 1 dx

Figure 6:

Strain Energy For a linear elastic material,

U

= 1 2

P

1

x

1 where P 1 is the value of the load corresponding to the deformation x 1 . (5) The units of energy are Joule (N.m) in SI units or in.lb in U.S. Customary units. The strain energy is dependent on the length and cross-sectional area of the test specimen. Strain energy density or strain energy per unit volume is independent of the dimensions of the specimen.

Strain energy density

is actually the area under the stress strain curve.

Resilience

The strain energy density at be expressed as

yield

is known as the resilience modulus. Resilience is the capacity of a material to absorb energy elastically upon loading. Mathematically, this can ε

y U r

= ∫ 0 σ

d

ε (6) The

modulus of resilience

represents the energy per unit volume that the material can absorb without yielding. Figure 7 shows that for a linear elastic material

U r

= ∫ 0 ε

y

σ

d

ε = 0 .

5 σ

y

ε

y

= σ 2

y

2

E

9/24/2004 6

CIE 361 Fall 2004 σ σ Y Y Instructor: Christine Human Modulus of resilience ε Y ε

0.0002 Figure 7:

modulus of resilience Units of resilience are joules per cubic meter or inch-pounds force per cubic inch. Resilient materials have a high yield strength and a low modulus of elasticity, properties useful for components such as springs. The capacity of a structure to withstand an impact load without being permanently deformed also depends on its resilience,

Toughness

Qualitatively, the toughness is the strain energy density (area under the stress-strain curve) up to the point of

fracture

(see Figure 8 ) and is given by: ε

f

∫ 0 σ

d

ε (8) The units for toughness are the same as those for resilience (energy per unit volume). Similar to the calculation of resilience, the toughness of a material can be determined from numerical integration of the stress-strain data. For a material to be considered tough, it must possess significant ductility and strength. Why? 9/24/2004 7

CIE 361 Fall 2004 σ Modulus of toughness Instructor: Christine Human Rupture

0.0002

ε f ε

Figure 8:

Toughness

Fracture

Fracture is the separation of a body into two or more parts. Two modes of fracture are possible, ductile or brittle.

The classification is based on whether the material can sustain substantial plastic deformation. Consider the three fractured specimens shown in Figure 9.

Figure 9:

Types of fracture (from Callister) a point. from steel specimens) Part (a) of the figure shows a highly ductile fracture in which the specimen necks down to Part (b) of the figure shows a moderately ductile fracture after some necking (expected Part (c) of the figure shows brittle fracture without any plastic deformation. 9/24/2004 8

CIE 361 Fall 2004 Instructor: Christine Human The Figure 10 (Callister(2000) shows the progression of fracture for a material which shows moderately ductile failure. Five stages in the cup-and cone fracture are shown. (a) (b) (c) (d) (e)

Figure 10:

Fracture of moderately ductile material Initial necking of the specimen Small cavities or micro voids from in the interior of the cross section Micro voids enlarge, come together, and coalesce to form an elliptical crack, which has its long axis perpendicular to the stress direction.

Crack continues to grow Fracture is preceded by the rapid propagation of a crack around the outer perimeter of the neck and by shear deformation at an angle of 45 degrees to the tension axis (the angle at which the shear stresses are maximum).

In contrast to the cup and cone fracture of a ductile material, a brittle material tends to fail along a horizontal plane where the normal stresses are a maximum.

### References

Callister, W.D.

Materials Science and Engineering

, 5th ed., John Wiley and Sons, New York, 2000 9/24/2004 9